data_z00250120301r_pl_inc_mask_om75_bkg1
_audit_creation_date               2022-07-21
_audit_creation_method
;
Olex2 1.5-ac5-023
(compiled 2022.04.12 svn.rca3783a0 for Rigaku Oxford Diffraction, GUI svn.r6498)
;
_shelx_SHELXL_version_number       '2018/3'
_audit_contact_author_address      ?
_audit_contact_author_email        ?
_audit_contact_author_name         ''
_audit_contact_author_phone        ?
_publ_contact_author_id_orcid      ?
_publ_section_references
;
Dolomanov, O.V., Bourhis, L.J., Gildea, R.J, Howard, J.A.K. & Puschmann, H.
 (2009), J. Appl. Cryst. 42, 339-341.

Sheldrick, G.M. (2015). Acta Cryst. A71, 3-8.

Sheldrick, G.M. (2015). Acta Cryst. C71, 3-8.
;
_chemical_name_common              ?
_chemical_name_systematic          ?
_chemical_formula_moiety           'Ga La O4 Sr'
_chemical_formula_sum              'Ga La O4 Sr'
_chemical_formula_weight           360.25
_chemical_melting_point            ?
_chemical_oxdiff_formula           'Sr La Ga O4'
loop_
  _atom_type_symbol
  _atom_type_description
  _atom_type_scat_dispersion_real
  _atom_type_scat_dispersion_imag
  _atom_type_scat_source
 'Ga' 'Ga' 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'La' 'La' -0.2871 2.4523
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O' 'O' 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Sr' 'Sr' -1.5307 3.2498
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system        'tetragonal'
_space_group_IT_number             139
_space_group_name_H-M_alt          'I 4/m m m'
_space_group_name_Hall             '-I 4 2'
loop_
  _space_group_symop_operation_xyz
 'x, y, z'
 '-x, -y, z'
 '-y, x, z'
 'y, -x, z'
 '-x, y, -z'
 'x, -y, -z'
 'y, x, -z'
 '-y, -x, -z'
 'x+1/2, y+1/2, z+1/2'
 '-x+1/2, -y+1/2, z+1/2'
 '-y+1/2, x+1/2, z+1/2'
 'y+1/2, -x+1/2, z+1/2'
 '-x+1/2, y+1/2, -z+1/2'
 'x+1/2, -y+1/2, -z+1/2'
 'y+1/2, x+1/2, -z+1/2'
 '-y+1/2, -x+1/2, -z+1/2'
 '-x, -y, -z'
 'x, y, -z'
 'y, -x, -z'
 '-y, x, -z'
 'x, -y, z'
 '-x, y, z'
 '-y, -x, z'
 'y, x, z'
 '-x+1/2, -y+1/2, -z+1/2'
 'x+1/2, y+1/2, -z+1/2'
 'y+1/2, -x+1/2, -z+1/2'
 '-y+1/2, x+1/2, -z+1/2'
 'x+1/2, -y+1/2, z+1/2'
 '-x+1/2, y+1/2, z+1/2'
 '-y+1/2, -x+1/2, z+1/2'
 'y+1/2, x+1/2, z+1/2'

_cell_length_a                     3.84230(10)
_cell_length_b                     3.84230(10)
_cell_length_c                     12.6752(5)
_cell_angle_alpha                  90
_cell_angle_beta                   90
_cell_angle_gamma                  90
_cell_volume                       187.127(12)
_cell_formula_units_Z              2
_cell_measurement_reflns_used      3796
_cell_measurement_temperature      301
_cell_measurement_theta_max        41.7240
_cell_measurement_theta_min        3.2080
_shelx_estimated_absorpt_T_max     ?
_shelx_estimated_absorpt_T_min     ?
_exptl_absorpt_coefficient_mu      32.416
_exptl_absorpt_correction_T_max    1.00000
_exptl_absorpt_correction_T_min    0.88742
_exptl_absorpt_correction_type     multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.30a (Rigaku Oxford Diffraction, 2021)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details     ?
_exptl_crystal_colour              colourless
_exptl_crystal_colour_primary      colourless
_exptl_crystal_density_diffrn      6.394
_exptl_crystal_density_meas        ?
_exptl_crystal_density_method      ?
_exptl_crystal_description         irregular
_exptl_crystal_F_000               316
_exptl_crystal_size_max            0.005
_exptl_crystal_size_mid            0.005
_exptl_crystal_size_min            0.004
_exptl_transmission_factor_max     ?
_exptl_transmission_factor_min     ?
_diffrn_reflns_av_R_equivalents    0.0267
_diffrn_reflns_av_unetI/netI       0.0065
_diffrn_reflns_Laue_measured_fraction_full  1.000
_diffrn_reflns_Laue_measured_fraction_max  1.000
_diffrn_reflns_limit_h_max         6
_diffrn_reflns_limit_h_min         -6
_diffrn_reflns_limit_k_max         6
_diffrn_reflns_limit_k_min         -6
_diffrn_reflns_limit_l_max         18
_diffrn_reflns_limit_l_min         -20
_diffrn_reflns_number              5418
_diffrn_reflns_point_group_measured_fraction_full  1.000
_diffrn_reflns_point_group_measured_fraction_max  1.000
_diffrn_reflns_theta_full          25.242
_diffrn_reflns_theta_max           36.189
_diffrn_reflns_theta_min           3.214
_diffrn_ambient_temperature        301
_diffrn_detector                   'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean   10.0000
_diffrn_detector_type              'HyPix-Arc 150'
_diffrn_measured_fraction_theta_full  1.000
_diffrn_measured_fraction_theta_max  1.000
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
--------------------------------------------------------------------------
  1  ω    -11.00  37.00   0.50   30.00    --   -0.59  19.00-180.00   96
  2  ω    -34.00   4.00   0.50   30.00    --   -0.59 -19.00   0.00   76
  3  ω      2.00  30.00   0.50   30.00    --   -0.59  93.00  20.75   56
  4  ω    -16.00  33.00   0.50   30.00    --   -6.00  18.00  97.93   98
  5  ω    -21.00   4.00   0.50   30.00    --   -6.00  13.00  88.13   50
  6  ω    -11.00  14.00   0.50   30.00    --   -0.59  19.00 -30.00   50
  7  ω    -11.00  23.00   0.50   30.00    --   -0.59  19.00-150.00   68
  8  ω    -41.00 -15.00   0.50   30.00    --   -0.59 -33.00 -49.60   52
  9  ω    -11.00  14.00   0.50   30.00    --   -0.59  19.00   0.00   50
 10  ω    -11.00  14.00   0.50   30.00    --   -0.59  19.00 150.00   50
 11  ω    -11.00  37.00   0.50   30.00    --   -0.59  19.00  30.00   96
 12  ω    -15.00  31.00   0.50   30.00    --   -0.59  17.00-118.16   92
 13  ω      2.00  29.00   0.50   30.00    --   -0.59  88.00 -18.85   54
 14  ω      0.00  30.00   0.50   30.00    --   -0.59  92.00  90.38   60
 15  ω     15.00  40.00   0.50   30.00    --   -0.59  34.00 -28.57   50
 16  ω    -27.00  -1.00   0.50   30.00    --   -0.59 -92.00 129.40   52
 17  ω     -9.00  30.00   0.50   30.00    --   -0.59  19.00 120.00   78
 18  ω     -2.00  27.00   0.50   30.00    --   -0.59  94.00-109.73   58
 19  ω     -4.00  23.00   0.50   30.00    --   -6.00  89.00 -37.89   54
 20  ω     -3.00  31.00   0.50   30.00    --   -6.00  23.00 156.17   68
 21  ω    -21.00  19.00   0.50   30.00    --   -6.00  17.00  76.24   80
 22  ω    -10.00  19.00   0.50   30.00    --   -6.00  21.00 -64.67   58
 23  ω     -4.00  25.00   0.50   30.00    --   -6.00  93.00 157.47   58
 24  ω      3.00  31.00   0.50   30.00    --   -6.00  26.00 -37.64   56
 25  ω    -19.00   7.00   0.50   30.00    --   -6.00  15.00 -77.43   52
;
_diffrn_measurement_device         'four-circle diffractometer'
_diffrn_measurement_device_type    'ROD, Synergy Custom system, HyPix-Arc 150'
_diffrn_measurement_method         'ω scans'
_diffrn_orient_matrix_type        
 'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11        0.0163643000
_diffrn_orient_matrix_UB_12        0.1826672000
_diffrn_orient_matrix_UB_13        0.0063351000
_diffrn_orient_matrix_UB_21        -0.1768584000
_diffrn_orient_matrix_UB_22        0.0099036000
_diffrn_orient_matrix_UB_23        0.0157416000
_diffrn_orient_matrix_UB_31        0.0502519000
_diffrn_orient_matrix_UB_32        -0.0246448000
_diffrn_orient_matrix_UB_33        0.0533343000
_diffrn_radiation_monochromator    mirror
_diffrn_radiation_probe            x-ray
_diffrn_radiation_type             'Mo K\a'
_diffrn_radiation_wavelength       0.71073
_diffrn_source                     'Rotating-anode X-ray tube'
_diffrn_source_type                'Rigaku (Mo) X-ray Source'
_reflns_Friedel_coverage           0.000
_reflns_Friedel_fraction_full      .
_reflns_Friedel_fraction_max       .
_reflns_number_gt                  162
_reflns_number_total               169
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression       'I > 2σ(I)'
_computing_cell_refinement         'CrysAlisPro 1.171.42.30a (Rigaku OD, 2021)'
_computing_data_collection         'CrysAlisPro 1.171.42.30a (Rigaku OD, 2021)'
_computing_data_reduction          'CrysAlisPro 1.171.42.30a (Rigaku OD, 2021)'
_computing_molecular_graphics      'Olex2 1.5-ac5-023 (Dolomanov et al., 2009)'
_computing_publication_material    'Olex2 1.5-ac5-023 (Dolomanov et al., 2009)'
_computing_structure_refinement    'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution      'SHELXT  (Sheldrick, 2015)'
_refine_diff_density_max           0.544
_refine_diff_density_min           -0.574
_refine_diff_density_rms           0.101
_refine_ls_extinction_coef         0.0011(2)
_refine_ls_extinction_expression  
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
_refine_ls_extinction_method       'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref     1.331
_refine_ls_hydrogen_treatment      undef
_refine_ls_matrix_type             full
_refine_ls_number_parameters       13
_refine_ls_number_reflns           169
_refine_ls_number_restraints       0
_refine_ls_R_factor_all            0.0078
_refine_ls_R_factor_gt             0.0068
_refine_ls_restrained_S_all        1.331
_refine_ls_shift/su_max            0.000
_refine_ls_shift/su_mean           0.000
_refine_ls_structure_factor_coef   Fsqd
_refine_ls_weighting_details      
 'w=1/[σ²(Fo²)+(0.0030P)²+0.2374P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme        calc
_refine_ls_wR_factor_gt            0.0144
_refine_ls_wR_factor_ref           0.0147
_refine_special_details            ?
_olex2_refinement_description
;
1. Shared sites
{Sr01, La01}
2. Uiso/Uaniso restraints and constraints
Uanis(Sr01) = Uanis(La01)
3. Others
 Fixed Sof: Sr01(0.0625) La01(0.0625)
;
_atom_sites_solution_hydrogens     .
_atom_sites_solution_primary       dual
_atom_sites_solution_secondary     ?
loop_
  _atom_site_label
  _atom_site_type_symbol
  _atom_site_fract_x
  _atom_site_fract_y
  _atom_site_fract_z
  _atom_site_U_iso_or_equiv
  _atom_site_adp_type
  _atom_site_occupancy
  _atom_site_site_symmetry_order
  _atom_site_calc_flag
  _atom_site_refinement_flags_posn
  _atom_site_refinement_flags_adp
  _atom_site_refinement_flags_occupancy
  _atom_site_disorder_assembly
  _atom_site_disorder_group
 Sr01 Sr 0.000000 0.000000 0.35857(2) 0.00628(5) Uani 0.5 8 d S T P . .
 La01 La 0.000000 0.000000 0.35857(2) 0.00628(5) Uani 0.5 8 d S T P . .
 Ga01 Ga 0.000000 0.000000 0.000000 0.00719(8) Uani 1 16 d S T P . .
 O01 O 0.000000 0.500000 0.000000 0.0078(3) Uani 1 8 d S T P . .
 O02 O 0.000000 0.000000 0.16716(17) 0.0149(4) Uani 1 8 d S T P . .


_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
  _geom_bond_atom_site_label_1
  _geom_bond_atom_site_label_2
  _geom_bond_distance
  _geom_bond_site_symmetry_2
  _geom_bond_publ_flag
 Sr01 Ga01 3.25505(13) 9_455 ?
 Sr01 Ga01 3.25505(13) 9_445 ?
 Sr01 Ga01 3.25505(13) 9 ?
 Sr01 O01 2.62765(14) 9_545 ?
 Sr01 O01 2.62765(14) 9_445 ?
 Sr01 O01 2.62765(14) 11 ?
 Sr01 O01 2.62765(14) 11_545 ?
 Sr01 O02 2.7364(3) 25_455 ?
 Sr01 O02 2.7364(3) 25_445 ?
 Sr01 O02 2.7364(3) 25_545 ?
 Sr01 O02 2.426(2) . ?
 Sr01 O02 2.7364(3) 25 ?
 Ga01 O01 1.92115(5) 3_655 ?
 Ga01 O01 1.92115(5) 3 ?
 Ga01 O01 1.92115(5) 1_545 ?
 Ga01 O01 1.92115(5) . ?
 Ga01 O02 2.119(2) 17 ?
 Ga01 O02 2.119(2) . ?

loop_
  _geom_angle_atom_site_label_1
  _geom_angle_atom_site_label_2
  _geom_angle_atom_site_label_3
  _geom_angle
  _geom_angle_site_symmetry_1
  _geom_angle_site_symmetry_3
  _geom_angle_publ_flag
 Ga01 Sr01 Ga01 72.343(3) 9 9_455 ?
 Ga01 Sr01 Ga01 72.343(3) 9_445 9_455 ?
 Ga01 Sr01 Ga01 113.164(6) 9 9_445 ?
 O01 Sr01 Ga01 36.172(2) 9_445 9_445 ?
 O01 Sr01 Ga01 36.172(2) 9_445 9_455 ?
 O01 Sr01 Ga01 36.172(2) 11_545 9_445 ?
 O01 Sr01 Ga01 36.172(2) 11 9_455 ?
 O01 Sr01 Ga01 36.172(2) 11 9 ?
 O01 Sr01 Ga01 36.172(2) 9_545 9 ?
 O01 Sr01 Ga01 93.198(5) 11_545 9 ?
 O01 Sr01 Ga01 93.198(5) 11 9_445 ?
 O01 Sr01 Ga01 93.198(5) 9_545 9_455 ?
 O01 Sr01 Ga01 93.198(5) 9_445 9 ?
 O01 Sr01 Ga01 93.198(5) 9_545 9_445 ?
 O01 Sr01 Ga01 93.198(5) 11_545 9_455 ?
 O01 Sr01 O01 62.261(4) 11 9_445 ?
 O01 Sr01 O01 93.962(7) 9_545 9_445 ?
 O01 Sr01 O01 62.261(4) 11 9_545 ?
 O01 Sr01 O01 62.261(4) 9_545 11_545 ?
 O01 Sr01 O01 62.261(4) 11_545 9_445 ?
 O01 Sr01 O01 93.962(7) 11 11_545 ?
 O01 Sr01 O02 126.48(3) 11_545 25_455 ?
 O01 Sr01 O02 126.48(3) 9_545 25_445 ?
 O01 Sr01 O02 64.41(4) 9_545 25_545 ?
 O01 Sr01 O02 126.48(3) 9_445 25 ?
 O01 Sr01 O02 126.48(3) 11 25_545 ?
 O01 Sr01 O02 126.48(3) 11_545 25 ?
 O01 Sr01 O02 64.41(4) 9_445 25_445 ?
 O01 Sr01 O02 64.41(4) 9_445 25_455 ?
 O01 Sr01 O02 126.48(3) 9_445 25_545 ?
 O01 Sr01 O02 64.41(4) 11 25 ?
 O01 Sr01 O02 126.48(3) 11 25_445 ?
 O01 Sr01 O02 64.41(4) 11_545 25_445 ?
 O01 Sr01 O02 64.41(4) 11_545 25_545 ?
 O01 Sr01 O02 64.41(4) 9_545 25 ?
 O01 Sr01 O02 64.41(4) 11 25_455 ?
 O01 Sr01 O02 126.48(3) 9_545 25_455 ?
 O02 Sr01 Ga01 153.43(4) 25 9_445 ?
 O02 Sr01 Ga01 123.418(3) . 9_455 ?
 O02 Sr01 Ga01 93.76(2) 25_545 9 ?
 O02 Sr01 Ga01 93.76(2) 25 9_455 ?
 O02 Sr01 Ga01 123.418(3) . 9 ?
 O02 Sr01 Ga01 93.76(2) 25_455 9_445 ?
 O02 Sr01 Ga01 40.26(4) 25_455 9_455 ?
 O02 Sr01 Ga01 153.43(4) 25_545 9_455 ?
 O02 Sr01 Ga01 40.26(4) 25 9 ?
 O02 Sr01 Ga01 93.76(2) 25_545 9_445 ?
 O02 Sr01 Ga01 123.418(3) . 9_445 ?
 O02 Sr01 Ga01 153.43(4) 25_445 9 ?
 O02 Sr01 Ga01 93.76(2) 25_445 9_455 ?
 O02 Sr01 Ga01 93.76(2) 25_455 9 ?
 O02 Sr01 Ga01 40.26(4) 25_445 9_445 ?
 O02 Sr01 O01 133.019(3) . 9_445 ?
 O02 Sr01 O01 133.019(3) . 9_545 ?
 O02 Sr01 O01 133.019(3) . 11_545 ?
 O02 Sr01 O01 133.019(3) . 11 ?
 O02 Sr01 O02 166.31(9) 25_455 25_545 ?
 O02 Sr01 O02 89.186(11) 25_445 25_545 ?
 O02 Sr01 O02 83.16(4) . 25_545 ?
 O02 Sr01 O02 83.16(4) . 25_455 ?
 O02 Sr01 O02 166.31(9) 25_445 25 ?
 O02 Sr01 O02 89.186(11) 25_445 25_455 ?
 O02 Sr01 O02 83.16(4) . 25_445 ?
 O02 Sr01 O02 89.186(11) 25 25_545 ?
 O02 Sr01 O02 83.16(4) . 25 ?
 O02 Sr01 O02 89.186(11) 25 25_455 ?
 Sr01 Ga01 Sr01 113.163(6) 9_454 9_544 ?
 Sr01 Ga01 Sr01 72.343(3) 9_444 9_454 ?
 Sr01 Ga01 Sr01 72.343(3) 9_444 9_544 ?
 Sr01 Ga01 Sr01 180.0 9_554 25_445 ?
 Sr01 Ga01 Sr01 107.657(3) 25_445 9_454 ?
 Sr01 Ga01 Sr01 66.837(6) 9_444 25_445 ?
 Sr01 Ga01 Sr01 72.343(3) 9_554 9_454 ?
 Sr01 Ga01 Sr01 180.0 9_444 25 ?
 Sr01 Ga01 Sr01 113.163(6) 9_444 9_554 ?
 Sr01 Ga01 Sr01 107.657(3) 25 9_454 ?
 Sr01 Ga01 Sr01 66.837(6) 25 9_554 ?
 Sr01 Ga01 Sr01 107.657(3) 25 9_544 ?
 Sr01 Ga01 Sr01 107.657(3) 25_445 9_544 ?
 Sr01 Ga01 Sr01 113.163(6) 25 25_445 ?
 Sr01 Ga01 Sr01 72.343(3) 9_554 9_544 ?
 O01 Ga01 Sr01 126.171(1) . 25_445 ?
 O01 Ga01 Sr01 53.829(2) 3 9_454 ?
 O01 Ga01 Sr01 126.171(1) . 9_444 ?
 O01 Ga01 Sr01 126.171(2) 3 9_544 ?
 O01 Ga01 Sr01 126.171(1) 3_655 9_444 ?
 O01 Ga01 Sr01 53.829(1) 3_655 25 ?
 O01 Ga01 Sr01 53.829(2) . 9_454 ?
 O01 Ga01 Sr01 53.829(2) 3 25_445 ?
 O01 Ga01 Sr01 126.171(2) 1_545 9_454 ?
 O01 Ga01 Sr01 53.829(2) . 9_554 ?
 O01 Ga01 Sr01 53.829(1) . 25 ?
 O01 Ga01 Sr01 53.829(2) 1_545 25_445 ?
 O01 Ga01 Sr01 126.171(1) 3_655 9_454 ?
 O01 Ga01 Sr01 53.829(2) 3_655 9_544 ?
 O01 Ga01 Sr01 53.829(2) 1_545 9_544 ?
 O01 Ga01 Sr01 126.171(1) 1_545 25 ?
 O01 Ga01 Sr01 126.171(1) 3_655 25_445 ?
 O01 Ga01 Sr01 126.171(1) 3 25 ?
 O01 Ga01 Sr01 126.171(1) 3 9_554 ?
 O01 Ga01 Sr01 53.829(1) 3 9_444 ?
 O01 Ga01 Sr01 126.171(1) 1_545 9_554 ?
 O01 Ga01 Sr01 53.829(1) 1_545 9_444 ?
 O01 Ga01 Sr01 53.829(2) 3_655 9_554 ?
 O01 Ga01 Sr01 126.171(1) . 9_544 ?
 O01 Ga01 O01 90.0 3_655 . ?
 O01 Ga01 O01 90.0 3_655 1_545 ?
 O01 Ga01 O01 180.0 . 1_545 ?
 O01 Ga01 O01 90.0 3 1_545 ?
 O01 Ga01 O01 90.0 . 3 ?
 O01 Ga01 O01 180.0 3_655 3 ?
 O01 Ga01 O02 90.0 1_545 . ?
 O01 Ga01 O02 90.0 . . ?
 O01 Ga01 O02 90.0 1_545 17 ?
 O01 Ga01 O02 90.0 3_655 . ?
 O01 Ga01 O02 90.0 3 17 ?
 O01 Ga01 O02 90.0 3 . ?
 O01 Ga01 O02 90.0 3_655 17 ?
 O01 Ga01 O02 90.0 . 17 ?
 O02 Ga01 Sr01 123.419(3) . 9_454 ?
 O02 Ga01 Sr01 56.581(3) . 25_445 ?
 O02 Ga01 Sr01 56.581(3) 17 9_454 ?
 O02 Ga01 Sr01 56.581(3) 17 9_554 ?
 O02 Ga01 Sr01 123.419(3) . 9_554 ?
 O02 Ga01 Sr01 123.419(3) 17 25_445 ?
 O02 Ga01 Sr01 56.581(3) . 25 ?
 O02 Ga01 Sr01 56.581(3) 17 9_544 ?
 O02 Ga01 Sr01 123.419(3) 17 25 ?
 O02 Ga01 Sr01 123.419(3) . 9_444 ?
 O02 Ga01 Sr01 56.581(3) 17 9_444 ?
 O02 Ga01 Sr01 123.419(3) . 9_544 ?
 O02 Ga01 O02 180.0 17 . ?
 Sr01 O01 Sr01 86.039(7) 25 9_554 ?
 Sr01 O01 Sr01 93.961(7) 25 25_455 ?
 Sr01 O01 Sr01 86.039(7) 9_454 25_455 ?
 Sr01 O01 Sr01 180.0 9_454 25 ?
 Sr01 O01 Sr01 180.0 9_554 25_455 ?
 Sr01 O01 Sr01 93.961(7) 9_454 9_554 ?
 Ga01 O01 Sr01 90.0 1_565 9_454 ?
 Ga01 O01 Sr01 90.0 1_565 25_455 ?
 Ga01 O01 Sr01 90.0 . 9_554 ?
 Ga01 O01 Sr01 90.0 . 9_454 ?
 Ga01 O01 Sr01 90.0 . 25 ?
 Ga01 O01 Sr01 90.0 . 25_455 ?
 Ga01 O01 Sr01 90.0 1_565 9_554 ?
 Ga01 O01 Sr01 90.0 1_565 25 ?
 Ga01 O01 Ga01 180.0 1_565 . ?
 Sr01 O02 Sr01 96.84(4) . 25_455 ?
 Sr01 O02 Sr01 166.31(9) 25_545 25_455 ?
 Sr01 O02 Sr01 166.31(9) 25_445 25 ?
 Sr01 O02 Sr01 89.187(11) 25_445 25_545 ?
 Sr01 O02 Sr01 89.187(11) 25 25_545 ?
 Sr01 O02 Sr01 96.84(4) . 25_445 ?
 Sr01 O02 Sr01 89.187(11) 25 25_455 ?
 Sr01 O02 Sr01 96.84(4) . 25_545 ?
 Sr01 O02 Sr01 96.84(4) . 25 ?
 Sr01 O02 Sr01 89.187(11) 25_445 25_455 ?
 Ga01 O02 Sr01 83.16(4) . 25_455 ?
 Ga01 O02 Sr01 83.16(4) . 25_545 ?
 Ga01 O02 Sr01 83.16(4) . 25_445 ?
 Ga01 O02 Sr01 180.0 . . ?
 Ga01 O02 Sr01 83.16(4) . 25 ?

_olex2_submission_special_instructions  'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- B-factor correction
;
_oxdiff_exptl_absorpt_empirical_full_max  1.530
_oxdiff_exptl_absorpt_empirical_full_min  0.859
